1 International Photoenergy, Article ID , 5 pages Research Article Thermal Characteristics of InGaN/GaN Flip-Chip Light Emitting Diodes with Diamond-Like Carbon Heat-Spreading Layers Pai-Yang Tsai, 1 Hou-Kuei Huang, 1 Chien-Min Sung, 2 Ming-Chi Kan, 2 and Yeong-Her Wang 1 1 Institute of Microelectronics, Department of Electrical Engineering, Advanced Optoelectronic Technology Center, National Cheng Kung University, Tainan 71, Taiwan 2 Department of Technology, RiteDia, Hsin Chu 33, Taiwan Correspondence should be addressed to Yeong-Her Wang; Received 6 February 214; Revised 23 April 214; Accepted 2 June 214; Published 18 June 214 Academic Editor: Nelson Tansu Copyright 214 Pai-Yang Tsai et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. The temperature-dependent optical, electrical, and thermal properties of flip-chip light emitting diodes (FCLEDs) with diamondlike carbon () heat-spreading layers were investigated. On the basis of the measured results in the 2 Cto1 Ctemperature range, a significant performance improvement can be achieved for FCLEDs with heat-spreading layers (-FCLED) compared with FCLEDs without heat-spreading layers (non--fcled). The external quantum efficiency (EQE) of the -FCLED improves by 9% at an injection current of 1 ma and a temperature of 1 C. The forward voltage and spectra variations are smaller than those of non--fcleds. The -FCLED provides high efficiency and high stability performance for high-power and high-temperature applications. 1. Introduction GaN-based light emitter diodes (LEDs) are widely used for automotive lighting, solid-state lighting, and as light engines for other illumination tools [1, 2]. LEDs should operate at high injection currents and employ a large chip size when used for high-power applications. Therefore, the generated heat in LED chip and package is significant and cannot be neglected. The chip characteristics of conventional lateral LEDs are limited by technical problems; that is, the sapphire substrate suffers from poor electric and thermal properties . For flip-chip LEDs (FCLED), both the p and n pads are attached to a high thermal conductivity substrate by eutectic bonding or solder bumps. However, the current crowding is still not improved because the current circuit of the p and n pads is almost the same as conventional lateral LEDs . Therefore, the generated heat in the hot spot of the current crowding area significantly degrades the electric and optical properties of a device. Diamond-like carbon () possesses high thermal conductivity, thermal diffusivity, and thermal radiation; furthermore, the coefficient of thermal expansion (CTE) of is similar to that of GaN. has very good thermal conductivity (6 W/mK) and thermal diffusivity (37 mm 2 /s), that is, 1.5 and 3.3 times higher than that of copper [5, 6]. The can be very effective for heat dissipation and hot spot removal. Therefore, the improves chip performance at high injection current densities [7, 8]. In this study, the was used as a heat-spreading layer between the mirror and eutectic material. For the fabricated -FCLEDs, the temperature-dependent chip performance was discussed and compared with a FCLED without a heat-spreading layer (non--fcled). 2. Experimental The schematic of the LED cross section is shown in Figure 1. The GaN LED epilayers were grown by metal-organic chemical vapor depositions onto (1) sapphire substrates. The LEDstructureconsistedofalow-temperature2nmthick GaN buffer layer, a 2 μm thickundopedganlayer,a2μm thick and highly conductive n-type GaN layer, an InGaN- GaN multiple-quantum-well (MQW) active layer, and a
2 2 International Photoenergy n-pad Sapphire GaN Reflector p-bonding pad n-bonding pad Ceramic substrate (a) Figure 1: (a) Schematics of the FCLED with heat-spreading layer. (b) Cross-sectional heat-spreading layer SEM image for FCLED..5 μm thick p-type GaN layer. A 1 1mm 2 square isolation structure was created by using an inductively coupled plasma etcher (ICP) for electrical isolation. The p-gan was etched by an ICP to expose the n-gan for electrode deposition. Cr/Pt/Au were deposited on the n-gan as n pads, and the Ni/Ag//Au metals were deposited on the p-gan film. These metals acted as the ohmic contact and reflective mirrors formed by electron beam (E-beam) evaporation. The SiO 2 film was used to passivate the sidewall of the LED device through plasma-enhanced chemical vapor deposition. The / (25nm/2nm) materials were used as heat-spreading layers by physical vapor deposition after passivation. The use of a -layer can increase the adhesion and electrical conductivity of the heat-spreading layer. Finally, /Ni/AuSn was used as the bonding material layer for die attachment. To measure the temperature dependent onthefcledcharacteristics,thefcledwasattachedtoa ceramic substrate by using AuSn eutectic bonding. The LED chip was loaded onto a thermal plate composed of a copper stage, thermoelectric cooler, and thermistor. The temperature ranged from 2 Cto1 Cformeasuring purposes. The optical, spectral, and electric characteristics were measured by using an integrated sphere at various heat sink temperatures. 3. Results and Discussion The performances of the split-wafer -FCLED and the non--fcled were investigated. The light output power, injection current, and forward voltage (L-I-V) characteristics at room temperature are shown in Figure 2. At35mA, the forward voltage (V F ) of the -FCLED is 2.88 V, whereas the forward voltage (V F ) of the non--fcled is 2.86 V. The current-voltage curves are almost the same. The light output power is mw for the -FCLED and 41.3 mw for the non--fcled. The corresponding wall-plug efficiencies (light output power/injection current forward voltage) of -FCLED and non--fcled at 35 ma are 41.1% and 4.1%, respectively. No significant difference was observed in the device performance of the -FCLED and non--fcled. The heat generated in the epilayers is almost the same. The light output power of the -FCLED is higher than the non--fcled at an injection current of 1, ma. (b) Forward voltage (V) Heat sink temperature =25 C FCLED Non--FCLED Forward current (ma) 1 Figure 2: L-I-V characteristics of the -VLED and non-- VLED. External quantum efficiency (a.u.) Heat sink temperature ( C) -FCLED 35 ma -FCLED 7 ma -FCLED 1 ma Light output power (mw) Non--FCLED 35 ma Non--FCLED 7 ma Non--FCLED 1 ma Figure 3: Three EQEs of the -FCLED and non--fcled as functions of the heat sink temperature at different injection currents (35, 7, and 1, ma). The can provide better thermal conductivity and thermal radiation. Furthermore, the heat of the MQW can be uniformly spread on the film and can be transferred to the ceramic substrate. The light output power can be further improved by using the heat-spreading layers at high injection currents. Figure 3 shows the external quantum efficiency (EQE, (light output power/h])/(injection current/e), where h is the Planck constant, ] is frequency, and e is the elementary charge) of the -FCLED and non--fcled as a function of the heat sink temperature at injection currents of 35, 7, and 1, ma. At an injection current of 35 ma
3 International Photoenergy Junction temperature ( C) Forward voltage (V) FCLED Non--FCLED Forward current (ma) FCLED Non--FCLED Heat sink temperature ( C) Figure 4: Junction temperature as a function of the injection current for the -FCLED and the non--fcled. Figure 5: The forward voltage as a function of the heat sink temperature at an injection current of 1, ma. and with a heat sink temperature of 2 C, the EQE of the -FCLED and non--fcled are 44.1% and 43.2%, respectively. The EQE of the -FCLED is slightly higher than the EQE of the non--fcled. At a heat sink temperature of 1 C, the EQE decreases to 38.6% and 37% for the -FCLED and non--fcled, respectively. The EQE of the -FCLED improves by 5%. The heat from the chipcanberemovedbytheheat-spreadinglayerand ceramic substrate. At an injection current of 1, ma and at a heat sink temperature of 2 C, the EQE of the - FCLED and non--led decreases by 37.7% and 36.9%, respectively. All sample efficiencies decrease with increasing heat sink temperature. The droop rate of the EQE for the -FCLED was lower than that of the non--fcled. The EQE of the non--fcled is 36.9% and decreased to 28.8% at 1, ma, thus indicating a droop rate of 21.9%. The droop rate of the -FCLED EQE is 16.5%. The effect of the heat-spreading layer on the light extraction performance of the FCLED is significant at high injection currents within a particular heat sink temperature range. The junction temperatures of the -FCLED and non- -FCLED are measured by the forward voltage method. Figure4 shows the junction temperature as a function of the injection current for the -FCLED and non--fcled. For the non--led, the junction temperatures are 7.5 and C at 35 and 1, ma, respectively. However, the -FCLED exhibited lower junction temperatures with 63.4 and C at 35 and 1, ma, respectively. Thus, a lower junction temperature is achieved for the - FCLED. This result can be attributed to the better thermal conductivity, thermal diffusivity, and thermal radiation of the.thehighthermaldiffusivitycaneffectivelyremove the generated heat and decrease temperature differences. Therefore, the heat generated at a junction is efficiently spread by the layer on the ceramic substrate. According to the Stefan-Boltzmann equation, the power of black body radiation may be calculated as T(K) 4 W/m 2,and the power radiated is about.15 W/cm 2.Thisvalueisabout 5% of the input power of devices. Figure 5 shows that the forward voltage changes according to the heat sink temperature. The forward voltage decreases with increasing heat sink temperature because of chip heating. At 1, ma, the forward voltage of the - FCLED decreases from 3.19 V to 3.3 V with increasing heat sink temperature from 2 Cto1 C. By contrast, the voltage for the non--fcled decreases from 3.19 V to 2.97 V. The energy band gap narrows with decreasing forward voltage becauseoftheinternallygeneratedheatofthechip.the forward voltage of the -FCLED slightly decreases with increasing heat sink temperature from 2 Cto1 C. This canbeattributedtothebetterthermaldissipationofthe heat-spreading layer. TheFCLEDwithaheat-spreadinglayercandecrease wavelength shifts with increasing heat sink temperature. The electroluminescence (EL) spectra of the -FCLED and non--fcled at various heat sink temperatures and at an injection current of 1, ma are shown in Figure 6. The EL intensities decrease with increasing heat sink temperature; this result may be caused by the heating of the chip. The increase in heat sink temperature decreases the energy band gap. The EL spectra are represented by a red shift (Figures 6(a) and 6(b)). The wavelength peak of the -FCLED is 448.4nmat2 C, and the EL spectra shifted to nm at 1 C. The wavelength shifted by 3.5 nm at heat sink temperatures of 2 Cto1 C. The wavelength peak of non- -FCLED is nm at 2 C and its EL spectra shifts to 452.1nmat1 C. The wavelength shifted by 3.9 nm in heat sink temperatures between 2 Cand1 C. To validate the effect of heat-spreading layers, each 1 random selected chips for -FCLED and non- -FCLED were adopted for the junction temperature measurement. As results show in Figure 7 at an injection
4 4 International Photoenergy 2 C 2 C 4 C 4 C Normalized EL intensity (a.u.) 6 C 8 C 1 C Normalized EL intensity (a.u.) 6 C 8 C 1 C Δλ = 3.5 nm Wavelength (nm) (a) Δλ = 3.9 nm Wavelength (nm) (b) Figure 6: Normalized EL spectra as a function of the heat sink temperature for the (a) -FCLED and (b) non--fcled with an injection current of 1 ma. Junction temperature ( C) #1 #2 #3 #4 #5 #6 #7 #8 #9 #1 -FCLED Non--FCLED Chip number Figure 7: Junction temperature measurements for 1 -FCLED and 1 non--fcled chips at an injection current of 1 ma. The chips were randomly selected. current of 1 ma, the FCLED with heat-spreading layer shows the lower junction temperature as compared to that of non--fcled. The trend is very consistent which indicates the role of the heat-spreading layers is very effective in heating dissipation and hot spot removal. The performance difference is unlikely to be related to the process variation. 4. Conclusions This paper demonstrates that the use of heat-spreading layers can improve the optical and thermal properties of FCLEDs. The temperature-dependent device performance of the -FCLED is significantly improved compared with the performance of the non--fcled. At an injection currentof1,ma,thelightoutputpowerandeqeare mw and 28.8% for the non--fcled. By contrast, the light output power and EQE increase to 1,6.3 mw and 31.5%, respectively, for the -FCLED. The forward voltage and EL spectra variations are smaller for the -FCLED. At heat sink temperatures between 2 Cand1 C, the forward voltage decreases by.17 V, which is less than the voltage for the non--fcled at an injection current of 1, ma. The EL spectra of the -FCLED show the red shift of only 3.5 nm. This shift is less than the shift of the non- -FCLED at.4 nm. These results demonstrate the stable optical, electrical, and thermal properties of FCLEDs in highpower or high-temperature applications. Conflict of Interests The authors declare that there is no conflict of interests regarding the publication of this paper. References  D. F. Feezell, J. S. Speck, S. P. Denbaars, and S. Nakamura, Semipolar (221) InGaN/GaN light-emitting diodes for highefficiency solid-state lighting, IEEE/OSA Display Technology,vol.9,no.4,pp ,213.
5 International Photoenergy 5  C.-T. Lee, U.-Z. Yang, C.-S. Lee, and P.-S. Chen, White light emission of monolithic carbon-implanted InGaN-GaN lightemitting diodes, IEEE Photonics Technology Letters, vol. 18, no. 19, pp , 26.  T. Egawa, B. Zhang, and H. Ishikawa, High performance of InGaN LEDs on (111) silicon substrates grown by MOCVD, IEEE Electron Device Letters, vol. 26, no. 3, pp , 25.  O. B. Shchekin, J. E. Epler, T. A. Trottier et al., High performance thin-film flip-chip InGaN-GaN light-emitting diodes, Applied Physics Letters,vol.89,no.7,ArticleID7119,26. K.M.Leung,A.C.Cheung,B.C.Liuetal., Measuring thermal conductivity of CVD diamond and diamond-like films on silicon substrates by holographic interferometry, Diamond and Related Materials,vol.8,no.8-9,pp ,1999.  C. M. Sung and M. C. Kan, Cold cathode fluorescence light with amorphous diamond coated electrodes, Nano Science and Technology Institute-Nanotech,vol.1,pp ,26.  P.Y.Tsai,H.K.Huang,C.-M.Sung,M.C.Kan,andY.H.Wang, InGaN/GaN vertical light-emitting diodes with diamondlike carbon/titanium heat-spreading layers, IEEE Electron Device Letters,vol.34,no.8,pp ,213.  R.H.Horng,K.C.Shen,C.H.en,S.C.Lin,andD.S.Wuu, Performance of Cu-plating vertical LEDs in heat dissipation using diamond-like carbon, IEEE Electron Device Letters, vol. 35,no.2,pp ,214.
6 International Medicinal Chemistry Photoenergy International Organic Chemistry International International Analytical Chemistry Advances in Physical Chemistry International Carbohydrate Chemistry Quantum Chemistry Submit your manuscripts at The Scientific World Journal International Inorganic Chemistry Theoretical Chemistry Spectroscopy Analytical Methods in Chemistry Chromatography Research International International Electrochemistry Catalysts Applied Chemistry Bioinorganic Chemistry and Applications International Chemistry Spectroscopy